 Nano Express
 Open Access
 Published:
Shockinduced breaking of the nanowire with the dependence of crystallographic orientation and strain rate
Nanoscale Research Letters volume 6, Article number: 291 (2011)
Abstract
The failure of the metallic nanowire has raised concerns due to its applied reliability in nanoelectromechanical system. In this article, the breaking failure is studied for the [100], [110], and [111] singlecrystal copper nanowires at different strain rates. The statistical breaking position distributions of the nanowires have been investigated to give the effects of strain rate and crystallographic orientation on microatomic fluctuation in the symmetric stretching of the nanowires. When the strain rate is less than 0.26% ps^{1}, macrobreaking position distributions exhibit the anisotropy of microatomic fluctuation. However, when the strain rate is larger than 3.54% ps^{1}, the anisotropy is not obvious because of strong symmetric shocks.
Introduction
In recent years, the metallic nanowires applied as nanoconnectors [1] and the active components of nanoelectromechanical system (NEMS) devices [2, 3] have attracted extensive interests owing to their special mechanical [4], thermal [5], electrical [6], and magnetic [7] properties. The approaches to investigate nanowires in experiments include using scanning tunneling microscopy (STM) [8, 9], atomic force microscopy (AFM) [10], transmission electron microscope (TEM) [11, 12], and mechanically controllable break junctions (MCBJ) [13, 14]. However, it is difficult to manipulate the deformation processes when the nanowires are applied in NEMS, because controlling the failure of the nanowires is a challenging thing due to their small scales. Hemker [15] proposed the reliability of NEMS would require a fundamental description of its deformation mechanism, which must be based on a corresponding solid understanding. In contrast, molecular dynamics (MD) simulation [16, 17], which solves Newton's equations of motion for a collection of interacting particle over a number of time steps, is an effective method to study the deformation and breaking failure processes of the metallic nanowires.
With the method of MD simulation, Koh and Lee [18] studied the strainrate effects on the tensile structure of platinum nanowire. Meanwhile, they [19] gave the mechanical behaviors of gold and platinum nanowires under different strain rates, which indicated that the displayed crystallineordered deformation of the nanowires was governed by the formation of a main dislocation plane at low strain rate. Ikeda et al. [20] proposed amorphization in nickel nanowire induced by high strain rate. These studies indicate strainrate effects on the deformation of the singlecrystal metallic nanowires. For the singlecrystal materials, we noticed that the plastic response in copper could occur rapidly [21, 22]. According to this point, studying the deformation and breaking failure of the copper singlecrystal nanowires shall be of vital importance for developing and processing the nanoscale systems based on metallic nanowires. In addition, anisotropies in singlecrystal materials will give rise to the dependence of crystallographic orientation. For example, Tsuru and Shibutani [23] showed copper had a much larger anisotropic factor than aluminum in terms of the loaddepth relation and stress distribution. Bringa et al. [24] proved singlecrystal copper had a marked anisotropic behavior in shock wave propagation. It is known that crystallographic orientation is related with structural anisotropy and symmetric stretching at different strain rates will generate different mechanical shocks, but we do not know which factor will dominate the deformation and the breaking failure mechanism of the nanowires? In order to make the question clear, we focused on the MD simulation investigation of the tensile deformation and breaking failure of the singlecrystal copper nanowires under the effects of crystallographic orientation and strain rate.
It is also worth noting that the nanowires not only behave as intrinsic properties like bulk materials, but also have their special microcosmic behaviors due to nanoscale effects. In our previous work [25, 26], the breaking uncertainty of the nanowire was found when the nanowire was stretched at different lengths and strain rates. The similar microscopic phenomena in experiments were also found in the metallic and the molecular junction conductance followed by a statistical distribution [27, 28]. In our study, we designed different initial equilibrium states to investigate statistically the [100], [110], and [111] singlecrystal copper nanowires. As shown in Figure 1, we propose a theoretical explanation for the relationship of microatomic fluctuation and macrobreaking position distribution based on symmetric stretching and structural anisotropy. We find microatomic fluctuation plays a critical role in the deformation of nanowires. At low strain rates, macrobreaking position distributions reflect anisotropic characters of the singlecrystal nanowires, whereas the anisotropic characters behave unobvious at high strain rates because shocks induced by strong symmetric stretching dominate the breaking failure at two ends of the nanowires.
Methodology
To reveal the relationship between anisotropy and symmetric mechanical shocks, MD simulations were performed to study a total samples of 14,400 (3 × 16 × 300) of the singlecrystal copper nanowires. The geometric models of facecentered cubic (FCC) were generated as a regular lattice along the [100], [110], and [111] crystallographic orientations, respectively. The geometric dimension of nanowires in the simulations was set as 5a × 5a × 15a (a stands for lattice constant, 0.362 nm for copper), corresponding to 1,500 atoms. For each orientation, total of 16 strain rates were set from 0.01 to 7.69% ps^{1}, corresponding to the absolute rates from 0.08 to 481.07 m/s in Table 1. Different and enough time was adopted to relax the singlecrystal copper nanowires to get 300 initial equilibrium states for one crystallographic orientation at each strain rate.
The singlecrystal copper nanowires were subjected to uniaxial strain by uniformly moving the top and bottom fixed layers in the zdirection (Figure 1). The strain (ε) was defined as ε = (ll _{0})/l _{0}, where l was the current stretching length and l _{0} was the length just after relaxation. Free boundary condition was adopted. The Verlet leapfrog algorithm was used for the integration of motion equations to obtain velocity and trajectories of atoms. NośeHoover thermostat [29–31] as a rescaling method of velocity maintains the system at 300 K. The interaction between copper atoms was described through embeddedatom method (EAM) potential function developed by Johnson [32–34], which could provide an effective description of the transition metals with the FCC structure. The total energy was given by:
where E is the total internal energy of the system, V is the pair potential between atoms i and j, and r _{ ij } is the distance between them, F(ρ _{ i } ) is the energy to embed atom i in an electron density ρ _{ i } , φ(r _{ ij } ) is the electron density at atom i due to atom j as a function of the distance r _{ ij } . The stress (σ) in zdirection was calculated by the Virial scheme [35] as following:
Where is the stress tensor of atoms α in the tensile direction (zaxis), Ω _{ i } is the volume of i atoms, m is the mass, and is the velocity component of atom i in the z direction. ϕ, F, ρ, and ƒ are parameters from EAM potential [32], which corresponding to the pair potential, the embedded energy, the electron density between the atom i or j and all other atoms, the electron density in r _{ ij } between atomic i and j, respectively. The first and second terms in the right side of the above equation represent the thermal effect and the atomic interactions, respectively. All the presented MD simulations and visualization process were performed with the selfdeveloped software NanoMD [36], the reliability of algorithms has been validated not only by a large amount of theoretical simulations [25, 26, 37–41], but also with the comparison to the experimental measurements [42, 43].
Results and discussions
It is shown in Figure 1 that macrobreaking position distributions of the nanowires are from the microatomic fluctuation of three crystallographic orientations at different strain rates and the ways of atomic fluctuation are related with deformation mechanism of the nanowires. With the MD simulations of the nanowires at the strain rates from 0.01 to 7.69% ps^{1}, Videos S1S3 in Additional files 1, 2 and 3 are selected to exhibit the representative deformation behaviors of the [100] singlecrystal copper nanowires at the strain rates of 0.01, 1.54, and 6.16% ps^{1}, respectively. At low strain rate of 0.01% ps^{1} (Video S1 in Additional file 1), the nanowire slips along (111) planes after the elastic deformation. In general, for the FCC closed pack structure, Burgers vectors exit along the <110> direction and induce the structure slip and reconstruct themselves along (111) planes. The slippage mechanism had been discussed in detail by Finbow et al. [44], who gave that the overall dislocation associated with slippage had a Burgers vectors given by (a _{0}/2) [] in the nanoscale wire. The process can be better described as a uniform slip in the [] direction of one (111) plane relative to the neighboring one. Slippage retains the crystalline order in the plastic deformation, and the linear atomic chains tend to occur near the middle of the nanowire because of symmetric stress. At 1.54% ps^{1} (Video S2 in Additional file 2), the obvious slippage allowing for reconstruction along (111) plane is not found and the nanowire shows superplasticic behavior with amorphous structures. At 6.16% ps^{1} (Video S3 in Additional file 3), the nanowire is more likely to break near the two ends because of local melted structures.
The deformation styles of the [100] singlecrystal copper nanowires are mainly slippage, amorphization, and local melted structures at low, middle, and high strain rates, respectively. The dependence of deformation characters at the applied strain rates is related with the microatomic fluctuation of crystalline structures. The degree of lattice order could be reflected by the maximum average potential energy per atom, which results from the breaking of metallic bonds in the tensile deformation process. Bond breaking is a direct consequence of atomic fluctuation overcoming the interatomic cohesive energy, which in turn causes the disordered fluctuation of atoms. When the nanowire stretches, the atoms under strong shocks overcome the interatomic cohesive energy to get a disordered amorphous state with the increase of the average potential energy per atom. Figure 2a shows the maximum average potential energy per atom at each strain rate from the statistical results, and the energy increases with the strain rate increasing before the high strain rate of 5.39% ps^{1}, but it exhibits a decreasing trend after the strain rate of 5.39% ps^{1}, attributing that symmetric shocks are so strong that the shock wave at such high strain rate (>5.39% ps^{1}) has some difficulties in propagating from the two ends to the middle of the nanowire. So the nanowire behaves as the local melted structures at the two ends and retains the order lattice within the nanowire. We can also see the corresponding breaking characters at the selected strain rates from the representative snapshots of the [100] singlecrystal copper nanowires at the breaking moment in Figure 2b.
In comparison with [100], the [110] singlecrystal copper nanowires behave as different deformation behaviors at the strain rates of 0.01, 1.54, and 6.16% ps^{1} (see Videos S4S6 in Additional files 4, 5 and 6). As shown in Video S4 in Additional file 4, the [110] nanowire prefers to maintain the crystallographic structure at low strain rate of 0.01% ps^{1}. The neck appears abruptly with the strain increasing, and the nanowires break accompanying with a few atoms in the disorder movement. This behavior is in agreement with the observations of Tavazza et al. [45] Because the preferred slip directions are identical to the tensile direction so the system has no ability to get the atomic rearrangement at lower strain rates. The nanowires remain a better crystal structures during the weak mechanical shocks at low strain rates. Increasing the strain rate will result in the increasing of atomic thermal motion, which facilitates the ductility of the materials. The deformation behavior in Video S5 (Additional file 5) shows that a local lattice reconstruction becomes predominant after the first yield point and the necking takes place at the positions of the lattice reconstruction. Unlike at the low and middle strain rates, the [110] nanowire at the strain rate of 6.16% ps^{1} (Video S6 in Additional file 6) exhibits superplasticity behavior with local disordered deformation. With the tension strain increasing, the [110] nanowire is more likely to break near the two ends of the nanowire due to the symmetric stress and local melted structures.
For the special deformation behaviors of the [111] singlecrystal copper nanowires at the strain rates of 0.01, 1.54, and 6.16% ps^{1} (see Videos S7S9 in Additional files 7, 8 and 9), the difference from [100] and [110] is that the deformation mechanism is the partial lattice rotation for the [111] nanowires. After the relaxing, the nanowire retains relative order lattice at the low strain rate of 0.01% ps^{1}, and the disorder crystal structures becomes obvious at the strain rate of 1.54% ps^{1}. When the strain rate is at 6.16% ps^{1}, the local disorder structures distribute at the two ends of the nanowires with the strain increasing, not at one side of 0.01% or 1.54% ps^{1}. In the stretching processes of the nanowires, the disorder crystal structures increase obviously with the strain rate increasing. The effects of strain rates on deformation structures could be reflected by the maximum average potential energy per atom in Figure S1 (Additional file 10), which increases generally for each crystallographic orientation with the strain rate increasing. Within the simulated strain rates, the [111], [100], and [110] nanowires have the lowest energy, the intermediate energy, and the highest energy, respectively, which are consistent with lattice plane energies in FCC metals [46, 47].
From the above results, the singlecrystal copper nanowires present various deformation behaviors at each crystallographic orientation. At low strain rates, clear slippage for [100] orientation occurs along the (111) planes. When the copper nanowires are stretched along the [110] orientation, the obvious lattice reconstruction becomes predominant after the first yielding point, whereas the [111] nanowires are partial lattice rotation in the deformation processes. However, at high strain rates, the nanowires always behave as local disorder structures at the two ends for each crystalline orientation. The dependence of deformation mechanism on strain rate and crystallographic orientation indicates that anisotropy behaves obvious at low strain rates, whereas unobvious at high strain rates due to strong symmetric stretching. Different deformation behaviors of the nanowires, which may be effectively evaluated by the mechanical property, are attributed to the different deformation mechanisms.
For the effect of the strain rate on the mechanical property, Figure 3a shows the typical stressstrain responses of the [100] singlecrystal copper nanowires at strain rates from 0.01 to 7.69% ps^{1} (to refer to strain rates in Table 1). Stress increases linearly with the strain increasing before the first yield point (the critical point between elastic and plastic deformation), which is consistent with elastic law (That is σ _{1} = Yε _{1}, σ _{1}, and ε _{1} are the first yield strain and stress, respectively. Y is Young's modulus.). When the stress decreases abruptly after the first yield point, the nanowire undergoes an irreversible deformation which indicates the beginning of plastic deformation. Subsequently, the yield cycle repeats continuously with a decreasing trend, and the yield cycle is over when the nanowires have no ability to maintain their structures and finally break. At low strain rates, the displayed periodic characters of the stressstrain responses imply the presence of the temporary stable state. By contrast, the periodicity at high strain rates is not obvious in the whole yield cycle.
For the dependence of crystallographic orientation, Figure 3b, c and 3d give the first yield stress, strain, and Young's modulus as a function of strain rate, respectively. Strain rates applied on the [100], [110], and [111] nanowires are all from 0.01 to 7.69% ps^{1}, and the average statistical result is from 300 samples for each strain rate. For the [100] singlecrystal copper nanowires, the first yield strain and stress both increase with the strain rate increasing. However, the first yield strain and stress are insensitive to the lower strain rate, whereas they are sensitive to the higher strain rate. Here, we named the divided range of strain rates as insensitive area (I), transitional area (II), and sensitive area (III). Young's modulus (Y) is defined by Sun [48] as the stress of a material divided by its strain in the elastic deformation region, which may be used to evaluate the mechanical strength of the nanowires. In the insensitive area of strain rates (I), the average Y fluctuates within its error, and it behaves as an increasing trend in the transition area of strain rates (II). While reaching the sensitive area of strain rates (III), Y abruptly increases in a line with the strain rate increasing, indicating the presence of the hardening effect. However, while comparing among [100], [110], and [111] crystallographic orientations, the mechanical properties of the [110] nanowires behave as different characters. It is attributed to the deformation mechanism and breaking behavior of the [110] nanowire at different strain rates, i.e., the [110] nanowire always prefers to maintain its crystallographic structure at low, middle, and high strain rates, respectively, (see Videos S4S6 in Additional files 4, 5 and 6), so the mechanical property behaves insensitively to strain rates. In general, the stress and the Y of the [110] are not sensitive to strain rates within the range of strain rates, but the Y of the [110] indicates the largest mechanical strength.
The structural anisotropy and symmetric stretching under different strain rates could bring different deformation mechanisms and mechanical properties, which could give insight into mechanical breaking failure and operation of metallic nanowires. If we could predict the deformation behaviors and the final breaking positions of the nanowires, the breaking failure could be controlled and the nanowires also could be strengthened near the breaking positions to avoid failure.
For example, in most cases, the final breaking positions of [100] occur at the central part of the nanowire at low strain rates, and the nanowires are apt to break at the two ends with the strain rate increasing. Using the [100] nanowire, the scheme in Figure 4a shows the relationships between macrobreaking position distribution and deformation mechanism induced by microatomic fluctuation. The statistical histograms of the breaking positions are fitted with Gaussian function, and the fitting peaks replace the most probable breaking position (MPBP) of the nanowires [25]. The MPBP is in the middle of the [100] nanowire at the insensitive area of strain rate (I), and the MPBP distributes at the two ends of the [100] nanowire at the sensitive area of strain rate (III), whereas the MPBP is in the middle or two ends of the [100] nanowire at the transition area of the strain rate (II). In detail, Figure 4b shows the MPBP distributions of the [100] nanowires at the strain rates from 0.01 to 7.69% ps^{1} (to refer to strain rates in Table 1). The breaking position distributions at three areas correspond to the stretching deformation processes of the nanowires in equilibrium state, quasiequilibrium state, and nonequilibrium state, respectively. At low strain rates, the slippage along (111) planes dominates the stretching deformation, and atomic fluctuation is in an equilibrium state. Strong shocks at high strain rates result in the superplastic behaviors and local melted structures, which induced atomic fluctuation in nonequilibrium state, whereas the atomic fluctuation in quasiequilibrium state brings irregular character of the MPBP distribution at the transition area of the strain rate (II). It reflects the microscopic uncertain property of nanoscale materials. Moreover, there is a transition among the equilibrium state, quasiequilibrium state, and nonequilibrium state, e.g., Figure 〈11〉 in Figure 4b belongs to quasiequilibrium state of nonequilibrium state.
Under the same simulation conditions of the [100] nanowires, the breaking position distributions of the [110] and [111] nanowires behave completely different at the strain rates from 0.01 to 7.69% ps^{1} (to refer to strain rates in Table 1). The breaking position distributions in Figure 4c show that the [110] nanowires would like to break at two ends of the nanowire at the low simulated strain rates, and the symmetric property of the breaking position distribution becomes obvious with the strain rates increasing. However, the [111] nanowires in Figure 4d show the breaking position exhibits a singlepeak distribution at the insensitive area of strain rate (I), and the symmetric distributions at the two ends of the nanowire gradually behave obvious with the strain rates increasing. From the influence of crystallographic anisotropy, we conclude the implied relationships in the scheme of Figure 1. When the symmetric stretching of the nanowire is applied at the low strain rates (less than 0.26% ps^{1}), microatomic fluctuation in equilibrium state brings the system enough ability to exhibit anisotropic characters of the crystal structures. Therefore, different deformation mechanisms for each crystallographic orientation exhibit various macrobreaking position distributions of the nanowires at low strain rates. When the symmetric stretching of the nanowire is applied at the high strain rates (larger than 3.54% ps^{1}), strong symmetric shocks dominate the deformation and breaking at the two ends of the nanowires. And the microatomic fluctuation has not enough ability to exhibit anisotropic characters of the crystal structures, thus, symmetric stretching results in macrobreaking position distributions at the two ends of nanowires.
For the microscopic behaviors of atoms under mechanical shocks, Holid and coworkers [49–51], Kadau et al. [52], and Bringa et al. [24] studied the shock wave propagation in solid materials and demonstrated its existence in nanoscale materials. Koh et al. [18, 19] and Liu et al. [25] used the strain wave propagation theory to predict the breaking position of the nanowires. The theory could be stated that, if shock is involved, the longitudinal shock wave velocity can be derived from the simplified wave equation given by U s = (Y/ρ)^{1/2}, Y is the Young's modulus and ρ is the average density of solid materials, which is estimated to be 8,900 kg/m^{3} for copper, and the most probable breaking position of the nanowires could be predicted and interpreted with the shock wave propagation theory, using the shock wave propagation distance d = U s × t = (Y/ρ)^{1/2} × t, and t is the required time to attain atomic break.
The microscopic mechanism of shock wave propagation in solids is inherently complex because the plastic flow is governed by the creation and motion of defects in the deformation of nanoscale materials. Meanwhile, with the statistical analysis of samples, we can find it is difficult to calculate exactly the fixed breaking position using the above shock wave propagation equation, especially for the breaking in the distributions of [100], [110], and [111] crystallographic orientations at the insensitive area of strain rates, and the uncertainty of [100] at the transitional area of strain rates. From microscopic viewpoint, mechanical shock is induced by symmetric stretching at different strain rates, and different mechanical shocks and anisotropies could affect the microatomic fluctuation, which could induce different ways of shock wave propagation. Mechanical shocks can disrupt the lattice order in the tensile deformation of the nanowires, attributing the concentrated and dispersed energy in shock wave propagation which is converted to the atomic kinetic energy, so the atomic bonds will break when the activated atoms have enough energy to overcome the atomic cohesive energy. At low strain rates, symmetric stretching retains the relative order lattice in the equilibrium state. In this state, microatomic fluctuation in anisotropic crystal structures mainly affect shock wave propagation in the stretching processes of the [100], [110], and [111] copper nanowires. Different styles of shock wave propagation for each crystallographic orientation make macrobreaking position distributions with various characters. At high strain rates, symmetric stretching in nonequilibrium state brings a large stress gradient, which induces the difficulty of shock wave propagation, so shock waves overlap at the two ends of the nanowires, which tend to break at the two ends without anisotropic behaviors. Thus, macrobreaking position distributions at the two ends of the nanowires show symmetric characters at high strain rates.
Conclusion
In summary, we have simulated the [100], [110], and [111] singlecrystal copper nanowires subjected to symmetric stretching at strain rates from 0.01 to 7.69% ps^{1}, and we have studied the deformation behaviors, mechanical properties, and their breaking position distributions. We find that: (i) at low strain rates, the [100], [110], and [111] crystallographic orientations behave as three deformation mechanisms, slippage, reconstruction, and rotation, respectively. Whereas, high strain rates easily induce their local melted structures at two ends of the nanowires; (ii) for the effect of strain rate on the mechanical properties of [100], [110], and [111] crystallographic orientations, [100] is obvious, [110] is not obvious, and [111] is between of them; (iii) the macrobreaking position distributions reflect the microatomic fluctuation during the symmetric stretching applied on the nanowires. When the strain rate is less than 0.26% ps^{1}, macrobreaking position distributions exhibit the structural anisotropy. However, the anisotropy is not obvious when the strain rate is larger than 3.54% ps^{1} because of the strong symmetric shocks.
Abbreviations
 AFM:

atomic force microscopy
 EAM:

embeddedatom method
 FCC:

facecentered cubic
 MCBJ:

mechanically controllable break junctions
 MD:

molecular dynamics
 MPBP:

most probable breaking position
 NEMS:

nanoelectromechanical system
 STM:

scanning tunneling microscopy
 TEM:

transmission electron microscope.
References
 1.
Wu B, Heidelberg A, Boland JJ: Mechanical properties of ultrahighstrength gold nanowires. Nat Mater 2005, 4: 525. 10.1038/nmat1403
 2.
Husain A, Hone J, Postma HWC, Huang XMH, Drake T, Barbic M, Scherer A, Roukes ML: Nanowirebased veryhighfrequency electromechanical resonator. Appl Phys Lett 2003, 83: 1240. 10.1063/1.1601311
 3.
Lieber CM: Nanoscale science and technology: Building a big future from small things. MRS Bull 2003, 28: 486. 10.1557/mrs2003.144
 4.
Diao JK, Gall K, Dunn ML: Surfacestressinduced phase transformation in metal nanowires. Nat Mater 2003, 2: 656. 10.1038/nmat977
 5.
Miao L, Bhethanabotla VR, Joseph B: Melting of Pd clusters and nanowires: A comparison study using molecular dynamics simulation. Phys Rev B 2005, 72: 134109. 10.1103/PhysRevB.72.134109
 6.
Melosh NA, Boukai A, Diana F, Gerardot B, Badolato A, Petroff PM, Heath JR: Ultrahighdensity nanowire lattices and circuits. Science 300: 112. 10.1126/science.1081940
 7.
Alexandrov AS, Kabanov VV: Magnetic quantum oscillations in nanowires. Phys Rev Lett 95: 076601. 10.1103/PhysRevLett.95.076601
 8.
Agrait N, Rodrigo JG, Sirvent C, Vieira S: AtomicScale Connective Neck Formation and Characterization. Phys Rev B 1993, 48: 8499. 10.1103/PhysRevB.48.8499
 9.
Landman U, Luedtke WD, Salisbury BE, Whetten RL: Reversible manipulations of room temperature mechanical and quantum transport properties in nanowire junctions. Phys Rev Lett 1996, 77: 1362. 10.1103/PhysRevLett.77.1362
 10.
Agrait N, Rubio G, Vieira S: PlasticDeformation of NanometerScale Gold Connective Necks. Phys Rev Lett 1995, 74: 3995. 10.1103/PhysRevLett.74.3995
 11.
Legoas SB, Galvao DS, Rodrigues V, Ugarte D: Origin of anomalously long interatomic distances in suspended gold chains. Phys Rev Lett 2002, 88: 076105. 10.1103/PhysRevLett.88.076105
 12.
Rodrigues V, Fuhrer T, Ugarte D: Signature of atomic structure in the quantum conductance of gold nanowires. Phys Rev Lett 2000, 85: 4124. 10.1103/PhysRevLett.85.4124
 13.
Muller CJ, Vanruitenbeek JM, Dejongh LJ: Conductance and Supercurrent Discontinuities in AtomicScale Metallic Constrictions of Variable Width. Phys Rev Lett 1992, 69: 140. 10.1103/PhysRevLett.69.140
 14.
Muller CJ, Vanruitenbeek JM, Dejongh LJ: ExperimentalObservation of the Transition from Weak Link to Tunnel Junction. Physica C 1992, 191: 485. 10.1016/09214534(92)90947B
 15.
Hemker KJ: Understanding how nanocrystalline metals deform. Science 2004, 304: 22. 10.1126/science.1097058
 16.
Allen MP, Tildesley DJ: Computer Simulation of Liquids. New York: Clarendon; 1997.
 17.
Rapaport DC: The Art of Molecular Dynamics Simulation. Cambridge: Cambridge University Press; 2004.
 18.
Koh SJA, Lee HP: Molecular dynamics simulation of size and strain rate dependent mechanical response of FCC metallic nanowires. Nalotechnology 2006, 17: 3451. 10.1088/09574484/17/14/018
 19.
Koh ASJ, Lee HP: Shockinduced localized amorphization in metallic nanorods with strainratedependent characteristics. Nano Lett 2006, 6: 2260. 10.1021/nl061640o
 20.
Ikeda H, Qi Y, Cagin T, Samwer K, Johnson WL, Goddard WA: Strain rate induced amorphization in metallic nanowires. Phys Rev Lett 1999, 82: 2900. 10.1103/PhysRevLett.82.2900
 21.
LoveridgeSmith A, Allen A, Belak J, Boehly T, Hauer A, Holian B, Kalantar D, Kyrala G, Lee RW, Lomdahl P, Meyers MA, Paisley D, Pollaine S, Remington B, Swift DC, Weber S, Wark JS: Anomalous elastic response of silicon to uniaxial shock compression on nanosecond time scales. Phys Rev Lett 2001, 86: 2349. 10.1103/PhysRevLett.86.2349
 22.
Meyers MA, Gregori F, Kad BK, Schneider MS, Kalantar DH, Remington BA, Ravichandran G, Boehly T, Wark JS: Laserinduced shock compression of monocrystalline copper: characterization and analysis. Acta Mater 2003, 51: 1211. 10.1016/S13596454(02)004202
 23.
Tsuru T, Shibutani Y: Anisotropic effects in elastic and incipient plastic deformation under (001), (110), and (111) nanoindentation of Al and Cu. Phys Rev B 2007, 75: 035415. 10.1103/PhysRevB.75.035415
 24.
Bringa EM, Cazamias JU, Erhart P, Stolken J, Tanushev N, Wirth BD, Rudd RE, Caturla MJ: Atomistic shock Hugoniot simulation of singlecrystal copper. J Appl Phys 2004, 96: 3793. 10.1063/1.1789266
 25.
Liu YH, Zhao JW, Wang FY: The Influence of Length on Shockinduced Breaking Behavior of Copper Nanowires. Phys Rev B 2009, 80: 115417. 10.1103/PhysRevB.80.115417
 26.
Wang DX, Zhao JW, Hu S, Yin X, Liang S, Liu YH, Deng SY: Where, and how, does a nanowire break? Nano Lett 2007, 7: 1208. 10.1021/nl0629512
 27.
Xu BQ, Tao NJJ: Measurement of singlemolecule resistance by repeated formation of molecular junctions. Science 2003, 301: 1221. 10.1126/science.1087481
 28.
Reddy P, Jang SY, Segalman RA, Majumdar A: Thermoelectricity in molecular junctions. Science 2007, 315: 1568. 10.1126/science.1137149
 29.
Nośe S: A MolecularDynamics Method for Simulations in the Canonical Ensemble. Mol Phys 1984, 52: 255. 10.1080/00268978400101201
 30.
Nośe S: A Unified Formulation of the Constant Temperature MolecularDynamics Methods. J Chem Phys 1984, 81: 511. 10.1063/1.447334
 31.
Hoover WG: Canonical Dynamics  Equilibrium PhaseSpace Distributions. Phys Rev A 1985, 31: 1695. 10.1103/PhysRevA.31.1695
 32.
Johnson RA: Analytic NearestNeighbor Model for Fcc Metals. Phys Rev B 1988, 37: 3924. 10.1103/PhysRevB.37.3924
 33.
Johnson RA: Alloy Models with the EmbeddedAtom Method. Phys Rev B 1989, 39: 12554. 10.1103/PhysRevB.39.12554
 34.
Johnson RA: Relationship between Defect Energies and EmbeddedAtomMethod Parameters. Phys Rev B 1988, 37: 6121. 10.1103/PhysRevB.37.6121
 35.
Wu HA: Molecular dynamics study of the mechanics of metal nanowires at finite temperature. Eur J Mech A 2006, 25: 370. 10.1016/j.euromechsol.2005.11.008
 36.
Zhao JW, Yin X, Liang S, Liu YH, Wang DX, Deng SY, Hou J: Ultralarge scale molecular dynamics simulation for nanoengineering. Chem Res Chin Univ 2008, 24: 367. 10.1016/S10059040(08)60077X
 37.
Zhao JW, Wang FY, Jiang LY, Yin X, Liu YH: Breaking Behavior of a Bicrystal Copper Nanowire Studied Using a Fourier Transformation Method. Acta Phys Chim Sin 2009, 25: 1835.
 38.
Liu YH, Wang FY, Zhao JW, Jiang LY, Kiguchi M, Murakoshi K: Theoretical investigation on the influence of temperature and crystallographic orientation on the breaking behavior of copper nanowire. Phys Chem Chem Phys 2009, 11: 6514. 10.1039/b902795e
 39.
Wang FY, Liu YH, Yin X, Wang N, Wang DX, Gao YJ, Zhao JW: The interface and surface effects of the bicrystal nanowires on their mechanical behaviors under uniaxial stretching. J Appl Phys 2010, 108: 074311. 10.1063/1.3477323
 40.
Wang FY, Liu YH, Zhu TM, Gao YJ, Zhao JW: Nanoscale interface of metals for withstanding momentary shocks of compression. Nanoscale 2010, 2: 2818. 10.1039/c0nr00333f
 41.
Wang FY, Gao YJ, Zhu TM, Zhao JW: Shockinduced breaking in the gold nanowire with the influence of defects and strain rates. Nanoscale 2011, 3: 1624. 10.1039/c0nr00797h
 42.
Zhao JW, Murakoshi K, Yin X, Kiguchi M, Guo Y, Wang N, Liang S, Liu H: Dynamic Characterization of the Postbreaking Behavior of a Nanowire. J Phys Chem C 2008, 112: 20088. 10.1021/jp8055448
 43.
Jiang LY, Yin X, Zhao JW, Liu HM, Liu YH, Wang FY, Zhu JJ: Theoretical Investigation on the Thermal Stability of Au Hollow NanoParticle. J Phys Chem C 2009, 113: 20193. 10.1021/jp905280g
 44.
Finbow GM, LyndenBell RM, McDonald IR: Atomistic simulation of the stretching of nanoscale metal wires. Mol Phys 1997, 92: 705. 10.1080/002689797169989
 45.
Tavazza F, Levine LE, Chaka AM: Elongation and breaking mechanisms of gold nanowires under a wide range of tensile conditions. J Appl Phys 2009, 106: 043522. 10.1063/1.3200957
 46.
Keblinski P, Wolf D, Phillpot SR, Gleiter H: Structure of grain boundaries in nanocrystalline palladium by molecular dynamics simulation. Scripta Mater 1999, 41: 631. 10.1016/S13596462(99)001426
 47.
Wolf D, Yamakov V, Phillpot SR, Mukherjee A, Gleiter H: Deformation of nanocrystalline materials by moleculardynamics simulation: relationship to experiments. Acta Mater 2005, 53: 1. 10.1016/j.actamat.2004.08.045
 48.
Sun CQ: Size dependence of nanostructures: Impact of bond order deficiency. Prog Solid State Chem 2007, 35: 1. 10.1016/j.progsolidstchem.2006.03.001
 49.
Holian BL, Straub GK: MolecularDynamics of ShockWaves in 3Dimensional Solids  Transition from Nonsteady to Steady Waves in Perfect Crystals and Implications for the RankineHugoniot Conditions. Phys Rev Lett 1979, 43: 1598. 10.1103/PhysRevLett.43.1598
 50.
Holian BL: Modeling ShockWave Deformation Via MolecularDynamics. Phys Rev A 1988, 37: 2562. 10.1103/PhysRevA.37.2562
 51.
Straub GK, Holian BL, Petschek RG: MolecularDynamics of ShockWaves in OneDimensional Chains .2. Thermalization. Phys Rev B 1979, 19: 4049. 10.1103/PhysRevB.19.4049
 52.
Kadau K, Germann TC, Lomdahl PS, Holian BL: Microscopic view of structural phase transitions induced by shock waves. Science 2002, 296: 1681. 10.1126/science.1070375
Acknowledgements
This project was supported by the National Natural Science Foundation of China (Grant Nos. 20821063, 20873063 and 51071084), National Basic Research Program of China (973 Program, Grant No. 2007CB936302 and 2010CB732400), the Natural Science Foundation of Jiangsu Province (BK2010389) and Specialized Research Fund for the Doctoral Program of Higher Education (SRFDP, 20070284007).
Author information
Additional information
Competing interests
The authors declare that they have no competing interests.
Authors' contributions
FW carried out the simulations, participated in the design of the study, performed the statistical analysis and drafted the manuscript. YG and TZ participated in discussions. JZ conceived of the study, and participated in its design and coordination. All authors read and approved the final manuscript.
Electronic supplementary material
Additional file 10:Figure S1. The maximum average potential energy per atom plotted against strain rates for the [100], [110], and [111] singlecrystal copper nanowires. Figure S2 The representative stressstrain relationship of the [110] copper nanowire at the strain rates of 0.01, 1.54, and 6.16% ps^{1}. Figure S3 The representative stressstrain relationship of the [111] copper nanowire at the strain rates of 0.01, 1.54, and 6.16% ps^{1}. Stressstrain response for [110] and [111] crystallographic orientation Figure S2 in Additional file 1 shows the typical stressstrain responses of the singlecrystal copper nanowire along the [110] orientation from the initial equilibrium state to complete breakage at the strain rates of 0.01, 1.54, and 6.16% ps^{1}. The stressstrain responses in Figure S2 (Additional file 1) correspond to the representative deformation behaviors of the [110] copper nanowire in Videos S4, S5, and S6 of Additional files 5, 6, and 7, respectively (see Videos S4S6 in Additional files 5, 6, 7). For all the stressstrain responses, stress increases linearly with an increase in strain before the first yield point. After the first yield point, the stress decreases abruptly indicating the nanowire undergoes the plastic deformation and the irreversible deformation begins. Subsequently, the yield cycles repeat continuously until the final breaking of the nanowire. From Figure S2 in Additional file 1, we can find that the first yield strain increases from 0.057 to 0.075 when the strain rates increase from 0.01 to 6.16% ps^{1}, moreover, the breaking strain also increases from 0.433 to 1.286. In general, the stressstrain curve could reflect the tensile process and deformation mechanism, which depend on crystallographic orientation and strain rate. As shown in Video S4 of Additional file 5, the [110] nanowire prefers to maintain the crystallographic structure at low strain rate of 0.01% ps^{1}. The neck appears abruptly with the strain increasing, and then the nanowire breaks accompanying with a few atoms in the disorder movement. It is because the preferred slip directions are identical to the tensile direction so that the system has no ability to get the atomic rearrangement at lower strain rates. Thus, the stressstrain curve behaves sharp stress peaks and few yield cycles in Figure S2a (Additional file 1). At the low strain rate, the copper nanowire remains a better crystal structures due to weak mechanical shocks. Rising strain rate would increase the atomic thermal motion, which facilitates the ductility of the materials during stretching. Therefore, the stressstrain response embodies the dependence of mechanical properties on the strain rates. For the stressstrain response at the middle strain rate of 1.54% ps^{1}, the stress peaks of the yield cycles in Figure S2b (Additional file 1) are not as sharp as the ones at low strain rate in Figure S2a (Additional file 1), and the tensile strain increases obviously at this condition. Meanwhile, Video S5 in Additional file 6 shows that a local lattice reconstruction becomes predominant after the first yield point, and necking takes place at these reconstruction positions. Unlike the low and middle strain rates, the stressstrain curve of the [110] orientation are separated by a large stress well at the strain rate of 6.16% ps^{1} (Figure S2c in Additional file 1). Before the first yielding point, the nanowire undergoes elastic stretching. After the first yielding point, a stress hardening over a relatively wide range of strain can be observed. Between the first and the second yielding points, a local lattice reconstruction process occurs and it spreads to the whole nanowire. In Figure S2c (Additional file 1), the stressstrain response corresponds to Video S6 in Additional file 7 which exhibits local disordered deformation and the superplasticity behaviors. With the tension strain increasing, it is more likely to break near the two ends of the nanowire. In comparison with the singlecrystal copper nanowire along the [110] orientation, Figure S3 in Additional file 1 shows the typical stressstrain properties of copper nanowires stretched along the [111] orientation, which is simulated at the strain rates of 0.01, 1.54, and 6.16% ps^{1}. At the first stretching stage, the stress increases almost linearly for all the nanowires, and then reaches a critical point. In this process, the nanowires experience elastic deformation just like that of the [110] orientation. We can also find that both the yielding strain and the breaking strain increase with the strain rate increasing. However, [111] are lower than [110] at low and middle strain rates, whereas at high strain rate, [111] is higher than [110]. (GIF 2 MB)
Authors’ original submitted files for images
Below are the links to the authors’ original submitted files for images.
Rights and permissions
About this article
Cite this article
Wang, F., Gao, Y., Zhu, T. et al. Shockinduced breaking of the nanowire with the dependence of crystallographic orientation and strain rate. Nanoscale Res Lett 6, 291 (2011) doi:10.1186/1556276X6291
Received
Accepted
Published
DOI
Keywords
 High Strain Rate
 Crystallographic Orientation
 Shock Wave Propagation
 Mechanical Shock
 Position Distribution